Volume LVI 15 Number 2, 2008

115

### DEFORMATION AND FRACTURE

### PROPERTIES OF DARK CHOCOLATE

### L. Severa

**Received: January 14, 2008**

**Abstract**

SEVERA, L.: *Deformation and fracture properties of dark chocolate. *Acta univ. agric. et silvic. Mendel. Brun.,
2008, LVI, No. 2, pp. 115–122

Series of mechanical tests (uniaxial compression test, Brasil test, plate bending test) with cylidrical specimens made from dark chocolate have been performed. The stress-strain dependence has been ploted and modeled using data from compression test. The strain behaviour of the chocolate was found to be far from the linear elastic strain. The linear elasticity is limited for the very small strains. The Brasil test led to the development of the tensile stress in the specimen and its cracking. The de-pendence of the tensile stress on the strain rate has been conﬁ rmed. Also the linearity of the force vs. displacement data received during plate bending test has been limited to the very small value of the displacemnt. Impact behaviour of the chocolate has been also evaluated. Falling of the specimen from deﬁ ned hight led to its fracture. This experiment has been simulated using LS DYNA 3D ﬁ nite element code.

chocolate, elastic properties, mechanical loading, numerical simulation

Chocolate belongs to products that contain sig-niﬁ cant amounts of fats. Such products include e.g. butter, margarine, and many spreads such as cream, cheases etc. The solid-like character of these mate-rials is mainly due to an underlying network of weakly attractive polycrystalline fat particles. These fat particles arise from an aggregation process of pri-mary triacylglycerol crystals into increasingly larger clusters until a three-dimensional network is formed (Narine and Marangoni, 1999). Many of the sensory attributes such as spreadability, mouthfeel, snap of chocolate, texture, etc., are dependent on the me-chanical strength of the underlying fat crystal net-work. In addition to this obvious industrial impor-tance, fat crystal networks form a particular class of so materials, which demonstrate a yield stress and viscoelastic properties, rendering these materi-als plastic. From a materimateri-als sciences point of view, these materials are also extremely important. These properties are also very important for the evaluation of the extrusion processes. This is why we can report a signiﬁ cant eﬀ orts to model the mechanical strength (Kamphuis and Jongschaap, 1985; Kamphuis et al., 1984; Nederveen, 1963; Papenhuijzen, 1971, 1972; Payne, 1964; Van den Tempel, 1961, 1979) of these

networks. A comprehensive model relating struc-tural network characteristics and solid/ liquid ratios of lipid networks to their mechanical strength is still missing.

In order to build up such model one must have available experimental data on the mechanical be-ha viour of these materials. The mecbe-hanical be be- ha-viour of the chocolate has been studied in many pa-pers (Marangoni and Narine 2002). These stu dies were mostly limited to the evaluation of the viscoe-lastic properties under vibration test. There is a li-mi ted number of paper dealing with the evaluation of some basic parameters like the Young modulus, Poisson ratio, mechanical strength etc. The only two papers on the given topics have been reported (Mini-ﬁ e 1989, Missaire et al.,1990).

In the given paper the following problems have been studied:

• evaluation of the elastic properties of the cho-colate

• description of the stress strain behaviour under diﬀ erent loading rates

• evaluation of the tensile strength.

nu-merical data have been compared with the experi-mental ones.

**MATERIAL AND EXPERIMENTAL **

**PROCEDURE**

For the experiments a commercially available LINDT chocolate Excellence 85% Cocoa has been used. The specimens in form of a cylinder (12 mm in diameter and 6 mm in height) have been prepared from this chocolate.

The specimens were loaded using TIRA test-ing machine. Two diﬀ erent experiments have been performed:

1. The uniaxial compression test when specimens were compressed at the diﬀ erent crosshead speeds – 1, 10 and 100 mm/min. The integrated so ware converted the force crosshead displacement to stress-strain data.

2. The Brasil test (Hondros, 1959), originally de ve lo-ped to characterise the tensile strength of concrete (Faihurst, 1964). The schematic of this experiment is shown in Fig. 1.

1:* Schematic of the Brasil test*

The specimen is loaded in pressure by the force P. The loading is converted to the tension. For the ten-sile stress in the middle of the specimen is given by the relation:

### 2

*P*

*σ*

*t*

### = —— ,

*π*

*DL*

where *D* is the specimen diameter and *L* is its
height.

3. In order to get the deeper insight on the chocolate behaviour the plate bending experiments have been performed. The schematic of this experi-ments is shown in Fig. 2.

2: *Schematic of the plate bending*

A circular plate of the chocolate (65 mm in
diame-ter, thickness *h* = 3 mm) is supported at the circle with
the radius *r1* = 60 mm. The plate is loaded by the steel
cylinder with the radius of 5 mm. Under assumption
on the linear elastic behaviour of the plate material
the governing equation has the form

### 1

*d*

### ⎧

*d*

### ⎡

### 1

*d*

### ⎛

*dw*

### ⎞

### ⎤

### ⎫

*p*

### (

*r*

### )

### — —–

### ⎨

### r —–

### ⎢

### — —–

### ⎜

*r*

### —–

### ⎟ ⎥ ⎬

### = ——,

* r dr *

### ⎩

* dr *

### ⎣

* r dr *

### ⎝

* dr *

### ⎠ ⎦ ⎭

*K*

where *w (r)* is the plate deﬂ ection and *K* is the plate
rigidity.

*Eh*

3
*K*

### = ————

### 12(1

### −

*ν*

2_{)}

*E* is the Young modulus and ν is the Poisson ratio,
*p(r)* is the pressure on the upper plate surface. For
the loading shown in the Fig. 2 the pressure is given
by:

*F*

*p*

### (

*r*

### ) = —– .

*πρ*

2
All experiments were performed at the room temperature.

**RESULTS AND DISCUSSION**

**COMPRESSION TEST**

### ∆

*h*

*ε*

### = —–

*h*

_{o}*F*

*σ*

### = —– ,

*A*

_{o}where ε is the engineering strain, *ho* is the original
height, ∆*h* is the change in the height, σ (t) is the
en-gineering stress at time (t), *Ao* is the initial cross –
sec-tion of the specimen. These data can be used for
the evaluation of the true strain and true stress
(Cal-zada and Peleg, 1978):

*ε _{true}* = ln(1 +

*ε*)

*σ _{true}* =

*σe*−

*ε*

_{.}The stress is calculated usually of the assumption
that there is a little or no change in volume of
cho-co la te during its cho-compression. The cho-compressibility
given by *dV/V* can be expressed as (Ferry, 1980):

### 1

*dV*

### — —– = 1

### −

### 2

*ν*

### .

*V*

*d*

*ε*

The example of the stress – strain dependence is given in Fig. 3.

3: *Stress – strain dependence*

It has been found that this dependence can be ﬁ t-ted by the polynom:

*σ*

### (

*MPa*

### ) =

*a*

*ε*

4_{ + }

_{b}

_{b}

_{ε}

3_{ε}

_{ + }

_{c}

_{c}

_{ε}

2_{ε}

_{ + }

_{d}

_{d}

_{ε}

_{ε}

_{.}

This dependence is valid for the all cross – head velocities. If we use instead of the cross – head ve lo-ci ty V the strain rate:

*∂ε*

*V*

*ε*

### ˙

### ≡

### —– = —

*∂*

*t*

*h*

the experimental data can be ﬁ tted by the Cowper – Symonds equation (Cowper and Simons, 1958):

1

### ⎧

### ⎛

*ε*

### ˙

### ⎞

*p*

_{⎫}

*σ*

### = (

*a*

*ε*

4_{ + }

_{b}

_{b}

_{ε}

3_{ε}

_{ + }

_{c}

_{c}

_{ε}

2_{ε}

_{ + }

_{d}

_{d}

_{ε}

_{ε}

_{) }

_{⎨}

_{1 + }

_{⎜}

_{ — }

_{⎟}

_{ }

_{⎬}

_{,}

### ⎩

### ⎝

*D*

### ⎠

### ⎭

where *p* and *D* are the material parameters. The
ana-ly sis of the experimental data leads to the following
values of the parameters:

*a* = −242,03 MPa, *b* = 216,46 MPa, *c* = −66,72 MPa, *d *=
8,6 MPa. *D* = 152 000 s−1_{ and }_{p}_{ = 2.18}

From the Fig. 3 it is obvious that the strain be-haviour of the chocolate is far from the linear elas-tic strain. The linear elaselas-ticity is limited for the very small strains, i.e. for ε → ∞. Instead of the true Young modulus we can obtain only its apparent value:

### ⎛

### ∂σ

### ⎞

### E =

### ⎜

_{⎝}

### —–

### ⎟

### |(

### ε

### = 0)

### ∂ε

### ⎠

**BRASILIAN TEST**

This experiment shown in the Fig. 1 leads to the de-velopment of the tensile stress in the specimen. This tensile stress can and does lead to the cracking of the specimen. This is shown in the Fig. 4.

The dependence of the tensile stress on the cross-head displacement is shown in the Fig. 5.

It may be shown that the tensile stress also de-pends on the strain rate. The more detail observa-tions have shown that the cracks started at the cross-head displacement about 2 mm independently on the strain rate. It means the tensile strength is strain rate dependent. In order to obtain some quantitative expression the next experiments are needed.

4: *Specimen of the chocolate a er the brasilian test. Crosshead *
*velocity: 10 mm/min.*

**PLATE BENDING EXPERIMENT**

The solution of the governing equation presented in the Chapter 2 – see Fig. 2 is:

5: *The inﬂ uence of the crosshead velocity on the tensile stress*

*F*

### ⎧

### ⎛

*r*

_{1}

### ⎞

### ⎫

*w*

### (

*r*

### ) =

### −

### ———

### ⎨

### 4

*ρ*

2_{ln }

_{⎜}

_{ — }

_{⎟}

_{ + 8}

_{ρ}

2_{ρ}

_{(}

_{r}

_{r}

12

### ln

*r*

1### −

*r*

2### ln

*ρ*

### ) + 5

*ρ*

4### −

### 4

*ρ*

2*r*

2### −

*r*

4### ⎬

### .

### 64

*πρ*

2_{K}

_{K}

_{⎩ }

_{⎝}

_{ρ}

_{ρ}

_{⎠ }

_{⎭}

During the experiment shown in the Fig. 2 the dis-placement is measured at the point r = 0. For this point we obtain:

*F*

### ⎧

### ⎛

*r*

_{1}

### ⎞

### ⎫

*w*

### =

### −

### ———

### ⎨

### 4

*ρ*

2_{ln }

### ⎜

_{ — }

### ⎟

_{ + 8}

_{ρ}

2_{ρ}

_{(}

_{r}

_{r}

12

### ln

*r*

1### −

*r*

2### ln

*ρ*

### )

### ⎬

### .

### 64

*πρ*

2_{K}

_{K}

_{⎩ ⎝}

_{ρ}

_{ρ}

_{⎠ }

_{⎭}

As it was mentioned this solution was obtained for the linear elastic deformation of the plate. As it is

shown in the Fig. 6 the dependence between force *F*
and the displacement *w* is non – linear. It can be ﬁ
t-ted by:

*F*

### =

*aw*

3_{ + }

_{bw}

2_{bw}

_{+ }

_{cw}

_{cw}

_{,}

where a = 0.9032 N/mm3_{; b= −2.9836 N/mm}2_{ and c = }

The linearity is limited to the very small value of the displacemnt. If we perform the derivation dF/dw we obtain:

*dF*

### 64

*πρ*

2_{K}

_{K}

### —–

## |

*w*

### = 0 =

*c*

### =

### −

### ————————————.

* dw*

### ⎛

*r*

_{1 }

### ⎞

### 4

*ρ*

2_{ln }

### ⎜

_{ — }

### ⎟

_{ +8}

_{ρ}

2_{ρ}

_{(}

_{r}

_{r}

12

### ln

*r*

1### −

*ρ*

2### ln

*ρ*

### )

### ⎝

*ρ*

### ⎠

If we use the value of E = 9 MPa (an average value for the used strain rate) we obtain the value of the Poisson ratio:

*ν*

### = 0.415

its value is relatively closed to 0.5 which corresponds to the non – compressible material.

It is obvious that the obtained data describe only some basic features of the strain behaviour. This behaviour is highly non – linear and probably also time dependent. In order to verify the reliability of the obtained material parameters some in de pen dent experiment has been performed. Its description is given in the following part of the paper.

**IMPACT BEHAVIOUR OF THE CHOCOLATE**

The chocolate products can be subjected to some impact during their transportation etc. For our ex-periments the usual form of the chocolate – see Fig. 7 has been loaded by the falling from the heigth of 1 m. The velocity 4.5 m/s corresponds to this heigth. A er impact the chocolate has been fractured as shown in the Fig. 8.

7: *Table of the chocolate used for the impact loading*

This experiment has been simulated using LS DYNA 3D ﬁ nite element code. The computational model of the chocolate shown in the Fig. 7 is shown in the Fig. 9. Owing to the symmetry only a half of the specimen has been considered.

A detail of the computational mesh is shown in the Fig. 10.

9: *Computational model*

10: *Detail of the computational mesh*

**SUMMARY**

**SOUHRN**

### Deformační a lomové chování tmavé čokolády

Byla provedena řada mechanických zkoušek (tlaková zkouška, brazilský test, zkouška průhybem) na válečkových vzorcích (průměr 12 mm a výška 6 mm) tmavé čokolády. Výsledky tlakových zkoušek vedly k sestrojení grafu závislosti napětí – deformace. Uvedená závislost byla též úspěšně modelo-vána pomocí Cowper – Symondsova vztahu. Bylo zjištěno, že deformační chování čokolády není li-neá rně závislé na napětí. Oblast lili-neární elasticity je omezena pouze na velmi nízké hodnoty napětí. Brazilský test vedl k vzniku tahového napětí ve vzorku a jeho následnému porušení. Byla potvrzena závislost napětí na rychlosti deformace. Také provedení testu průhybem vedlo k závěru, že lineární chování čokolády je omezeno na počátek zatěžování. I tento test byl modelován s uspokojivým vý-sledkem. Bylo studováno též chování čokolády při rázovém zatížení. Tabulky čokolády byly zatěžo-vány dopadem z deﬁ nované výšky. Uvedený test byl numericky simulován pomocí konečněprvkové metody programem LS DYNA 3D.

čokoláda, elastické vlastnosti, mechanické zatěžování, numerická simulace

**ACKNOWLEDGEMENTS**

The research has been supported by the Grant Agency of the Czech Academy of Sciences under Con-tract No. IAA201990701.

**REFERENCES**

COWPER, G. R. and SYMONDS, P. S., 1958: Strain Hardening and Strain Rate Eﬀ ects in the Impact Loading of Cantilever Beams, Brown Univ. Ap-plied Mathematics Report, p. 28

FAIRHURST, C., 1964: On the validity of the ‘‘Brazi-lian’’ test for brittle materials. Int J Rock Mech Min Sci, 1, 535–46

FERRY, J. D., 1980: Viscoelastic Properties of Poly-mers, 3rd ed. Wiley

HONDROS, G., 1959: The evaluation of Poisson’s ra-tio and the modulus of materials of a low tensile resistance by the Brazilian (indirect tensile) test with particular reference to concrete. Aust J Appl Sci, 10, 243–68

KAMPHUIS, H., JONGSCHAMP, R. J. J. and MI-JNLIE, P. F., 1984: A transient-network model de-scribing the rheological behaviour of concentra-ted dispersions. Rheol. Acta, 23, 329–344

KAMPHIUS, H. and JONGSCHAAP, R. J. J., 1985: The rheological behaviour of suspensions of fat particles in oil interpreted in terms of a transient-network model. Colloid Polymer Science, 263, 1008–1024

MARANGONIA, A. G. and NARINE, S. S., 2002: Identifying key structural indicators of mecha-nical strength in networks of fat crystals, Food Re-search International 35, 957–969

MINIFIE, B. W., 1989: Chocolate, cocoa and confec-tionery, Science and technology. London: Chap-man & Hall

MISSAIRE, F., QIU, G. and RAO, M. A., 1990: Re-search note yield stress of structured and unstruc-tured food suspensions, Journal of Texture Stu-dies, 21, 479–490

NARINE, S. S. and MARANGONI, A. G., 1999: Re-lating structure of fat crystal networks to mecha-nical properties: a review, Food Research Interna-tional 32, 227–248

NEDERVEEN, C. J., 1963: Dynamic mechanical be-havior of suspensions of fat particles in oil. Journal of Colloid and Interface Science, 18, 276–291 PAPENHUIJZEN, J. M. P., 1971: Superimposed

steady and oscillatory shear in dispersed systems. Rheol. Acta, 10, 493–502

PAPENHUIJZEN, J. M. P., 1972: The role of particle interactions in the rheology of dispersed systems. Rheol. Acta, 11, 73–88

PAYNE, A. R., 1964: The elasticity of carbon black networks. Journal of Colloid Science, 19, 744–754 VAN DEN TEMPEL, M., 1961: Mechanical

proper-ties of plastic-disperse systems at very small defor-mations. Journal of Colloid and Interface Science, 16, 284–296

VAN DEN TEMPEL, M.,1979: Rheology of concen-trated suspensions. Journal of Colloid and Inter-face Science, 71, 18–20

Address